Li<sub>4</sub>P<sub>2</sub>Se<sub>6</sub> - structure and properties.
Neuberger, Sven; Mathew, Neeshma; Adediwura, Sheyi Clement; Sanchez, Hector Javier Cortes; Schmedt Auf der Günne, Jörn; Dalton transactions (Cambridge, England : 2003) 54 (2025) 11996–12005; doi:10.1039/d5dt00227c

data_7719068
_publ_section_title
;
 Li<sub>4</sub>P<sub>2</sub>Se<sub>6</sub> - structure and properties.
;
_journal_issue                   31
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11996
_journal_page_last               12005
_journal_paper_doi               10.1039/d5dt00227c
_journal_volume                  54
_journal_year                    2025
_chemical_formula_moiety         'P4 Se12, 8 (Li)'
_chemical_formula_structural     'Li4 P2 Se6'
_chemical_formula_sum            'Li8 P4 Se12'
_chemical_formula_weight         1126.92
_chemical_name_common            'Tetralithium selenidodiphosphate'
_chemical_name_systematic        'Tetralithium selenidodiphosphate'
_chemical_properties_physical
'air-sensitive, moisture-sensitive, hygroscopic'
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_atom_type_scat_source
;
Default data set used by TOPAS Academic 7.1
(A. Cohelo, TOPAS_Academic, Version 7.1)
;
_audit_creation_method           'TOPAS ACADEMIC 7.1'
_audit_update_record
;
2025-06-23 deposited with the CCDC.	2025-07-09 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.8707(1)
_cell_length_b                   11.2115(1)
_cell_length_c                   6.45445(7)
_cell_measurement_temperature    298
_cell_measurement_theta_max      89.990
_cell_measurement_theta_min      5.000
_cell_volume                     1003.740(16)
_computing_molecular_graphics    'Diamond 4'
_computing_publication_material  'TOPAS ACADEMIC 7.1'
_computing_structure_refinement  'TOPAS ACADEMIC 7.1'
_diffrn_ambient_pressure         1
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  'STOE STADI P'
_diffrn_radiation_monochromator  Ge-111
_diffrn_radiation_polarisn_ratio 1.0
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a~1~'
_diffrn_radiation_wavelength     1.54056
_diffrn_reflns_number            436
_diffrn_reflns_theta_max         90.1
_diffrn_source                   'sealed X-ray tube'
_exptl_absorpt_coefficient_mu    28.1172(5)
_exptl_absorpt_correction_type   cylinder
_exptl_absorpt_process_details   '(A. Cohelo, TOPAS_Academic, Version 7.1)'
_exptl_crystal_density_diffrn    3.72870(7)
_exptl_crystal_description       microcrystalline
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  red-brown
_pd_char_particle_morphology     powder
_pd_meas_number_of_points        8500
_pd_proc_ls_prof_wR_factor       4.211
_pd_proc_number_of_points        8500
_refine_ls_goodness_of_fit_all   1.918
_refine_ls_matrix_type           full
_refine_ls_number_constraints    4
_refine_ls_number_parameters     53
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          3.244
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         1.918
_reflns_limit_h_max              12
_reflns_limit_h_min              0
_reflns_limit_k_max              10
_reflns_limit_k_min              0
_reflns_limit_l_max              5
_reflns_limit_l_min              0
_reflns_number_total             436
_cod_data_source_file            d5dt00227c4.cif
_cod_data_source_block           Li4P2Se6
_cod_depositor_comments          'Adding full bibliography for 7719068.cif.'
_cod_original_sg_symbol_H-M      PNMA
_cod_database_code               7719068
_solution_special_details
; 
?
;
_pd_proc_ls_prof_r_expected      2.195
_shelx_f_squared_multiplier      1